Download presentation

1
**TOPIC 3 STRUCTURE OF SOLIDS**

ISSUES TO ADDRESS... • How do atoms assemble into solid structures? • How does the density of a material depend on its structure? • When do material properties vary with the sample orientation?

2
**POLYCRYSTALLINE MATERIALS**

“Nuclei” form during solidification, each of which grows into crystals

3
**ENERGY AND PACKING • Dense, regular packing**

• Non dense, random packing Dense, regular-packed structures tend to have lower energy

4
SOME DEFINITIONS … Crystalline material: atoms situated in a repeating 3D periodic array over large atomic distances Amorphous material: material with no such order Hard sphere representation: atoms denoted by hard, touching spheres Reduced sphere representation Unit cell: basic building block unit (such as a flooring tile) that repeats in space to create the crystal structure; it is usually a parallelepiped or prizm

5
**METALLIC CRYSTALS • tend to be densely packed.**

• have several reasons for dense packing: -Typically, made of heavy element. -Metallic bonding is not directional; i.e., no restrictions as to the number and position of nearest-neighbor atoms -Nearest neighbor distances tend to be small in order to lower bond energy. • have the simplest crystal structures. We will look at four such structures...

6
**ATOMIC PACKING FACTOR Fill a box with hard spheres**

Packing factor = total volume of spheres in box / volume of box Question: what is the maximum packing factor you can expect? In crystalline materials: Atomic packing factor = total volume of atoms in unit cell / volume of unit cell (as unit cell repeats in space)

7
**ATOMIC PACKING FACTOR a R=0.5a**

close-packed directions contains 8 x 1/8 = 1 atom/unit cell Lattice constant • APF for a simple cubic structure = 0.52

8
**BODY CENTERED CUBIC STRUCTURE (BCC)**

• Coordination # = 8 • Close packed directions are cube diagonals. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing.

9
**ATOMIC PACKING FACTOR: BCC**

Adapted from Fig. 3.2, Callister 6e. • APF for a body-centered cubic structure = p3/8 = 0.68

10
**FACE CENTERED CUBIC STRUCTURE (FCC)**

• Coordination # = 12 • Close packed directions are face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing.

11
**ATOMIC PACKING FACTOR: FCC**

• APF for a body-centered cubic structure = p/(32) = 0.74 (best possible packing of identical spheres)

12
**HEXAGONAL CLOSE-PACKED STRUCTURE (HCP)**

Ideally, c/a = for close packing However, in most metals, c/a ratio deviates from this value

13
**COMPARISON OF CRYSTAL STRUCTURES**

Crystal structure coordination # packing factor close packed directions Simple Cubic (SC) cube edges Body Centered Cubic (BCC) body diagonal Face Centered Cubic (FCC) face diagonal Hexagonal Close Pack (HCP) hexagonal side

14
**THEORETICAL DENSITY, r Density = mass/volume**

mass = number of atoms per unit cell * mass of each atom mass of each atom = atomic weight/avogadro’s number

15
**Characteristics of Selected Elements at 20C**

Adapted from Table, "Charac- teristics of Selected Elements", inside front cover, Callister 6e.

16
**THEORETICAL DENSITY, r Example: Copper**

Data from Table inside front cover of Callister (see previous slide): • crystal structure = FCC: 4 atoms/unit cell • atomic weight = g/mol (1 amu = 1 g/mol) • atomic radius R = nm (1 nm = 10 cm) -7

17
**DENSITIES OF MATERIAL CLASSES**

metals > ceramic s polymer Why? Metals have... • close-packing (metallic bonding) • large atomic mass Ceramics have... • less dense packing (covalent bonding) • often lighter elements Polymers have... • poor packing (often amorphous) • lighter elements (C,H,O) Composites have... • intermediate values Data from Table B1, Callister 6e.

18
CRYSTAL SYSTEMS Based on shape of unit cell ignoring actual atomic locations Unit cell = 3-dimensional unit that repeats in space Unit cell geometry completely specified by a, b, c & a, b, g (lattice parameters or lattice constants) Seven possible combinations of a, b, c & a, b, g, resulting in seven crystal systems

19
CRYSTAL SYSTEMS

20
**STRUCTURE OF OTHER SYSTEMS**

• Structure of NaCl (Courtesy P.M. Anderson) • Structure of Carbon Graphite Diamond

21
**CRYSTALLOGRAPHIC POINTS, DIRECTIONS & PLANES**

In crystalline materials, often necessary to specify points, directions and planes within unit cell and in crystal lattice Three numbers (or indices) used to designate points, directions (lines) or planes, based on basic geometric notions The three indices are determined by placing the origin at one of the corners of the unit cell, and the coordinate axes along the unit cell edges

22
POINT COORDINATES Any point within a unit cell specified as fractional multiples of the unit cell edge lengths Position P specified as q r s; convention: coordinates not separated by commas or punctuation marks

23
**EXAMPLE: POINT COORDINATES**

Locate the point (1/4 1 ½) Specify point coordinates for all atom positions for a BCC unit cell Answer: 0 0 0, 1 0 0, 1 1 0, 0 1 0, ½ ½ ½, 0 0 1, 1 0 1, 1 1 1, 0 1 1

24
**CRYSTALLOGRAPHIC DIRECTIONS**

Defined as line between two points: a vector Steps for finding the 3 indices denoting a direction Determine the point positions of a beginning point (X1 Y1 Z1) and a ending point (X2 Y2 Z2) for direction, in terms of unit cell edges Calculate difference between ending and starting point Multiply the differences by a common constant to convert them to the smallest possible integers u, v, w The three indices are not separated by commas and are enclosed in square brackets: [uvw] If any of the indices is negative, a bar is placed in top of that index

25
COMMON DIRECTIONS

26
EXAMPLES: DIRECTIONS Draw a [1,-1,0] direction within a cubic unit cell Determine the indices for this direction Answer: [120]

27
**CRYSTALLOGRAPHIC PLANES**

Crystallographic planes specified by 3 Miller indices as (hkl) Procedure for determining h,k and l: If plane passes through origin, translate plane or choose new origin Determine intercepts of planes on each of the axes in terms of unit cell edge lengths (lattice parameters). Note: if plane has no intercept to an axis (i.e., it is parallel to that axis), intercept is infinity (½ ¼ ½) Determine reciprocal of the three intercepts (2 4 2) If necessary, multiply these three numbers by a common factor which converts all the reciprocals to small integers (1 2 1) The three indices are not separated by commas and are enclosed in curved brackets: (hkl) (121) If any of the indices is negative, a bar is placed in top of that index

28
**THREE IMPORTANT CRYSTAL PLANES**

29
**THREE IMPORTANT CRYSTAL PLANES**

Parallel planes are equivalent

30
**EXAMPLE: CRYSTAL PLANES**

Construct a (0,-1,1) plane

31
**FCC & BCC CRYSTAL PLANES**

Consider (110) plane Atomic packing different in the two cases Family of planes: all planes that are crystallographically equivalent—that is having the same atomic packing, indicated as {hkl} For example, {100} includes (100), (010), (001) planes {110} includes (110), (101), (011), etc.

32
**LINEAR & PLANAR DENSITIES**

Linear density (LD) = number of atoms centered on a direction vector / length of direction vector LD (110) = 2 atoms/(4R) = 1/(2R) Planar density (PD) = number of atoms centered on a plane / area of plane PD (110) = 2 atoms / [(4R)(2R2)] = 2 atoms / (8R22) = 1/(4R22) LD and PD are important considerations during deformation and “slip”; planes tend to slip or slide along planes with high PD along directions with high LD

33
**CRYSTALS AS BUILDING BLOCKS**

• Single crystal: when the periodic and repeated arrangement of atoms is perfect and extends throughout the entirety of the specimen • Some engineering applications require single crystals: --diamond single crystals for abrasives --turbine blades Fig. 8.30(c), Callister 6e. (Fig. 8.30(c) courtesy of Pratt and Whitney). (Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.) • Crystal properties reveal features of atomic structure. --Ex: Certain crystal planes in quartz fracture more easily than others. (Courtesy P.M. Anderson)

34
**POLYCRYSTALLINE MATERIALS**

“Nuclei” form during solidification, each of which grows into crystals

35
**POLYCRYSTALS • Most engineering materials are polycrystals. 1 mm**

Adapted from Fig. K, color inset pages of Callister 6e. (Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany) 1 mm • Nb-Hf-W plate with an electron beam weld. • Each "grain" is a single crystal. • If crystals are randomly oriented, overall component properties are not directional. • Crystal sizes typ. range from 1 nm to 2 cm (i.e., from a few to millions of atomic layers).

36
**SINGLE VS POLYCRYSTALS**

• Single Crystals -Properties vary with direction: anisotropic. Data from Table 3.3, Callister 6e. (Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989.) -Example: the modulus of elasticity (E) in BCC iron: • Polycrystals 200 mm -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (Epoly iron = 210 GPa) -If grains are textured, anisotropic. Adapted from Fig. 4.12(b), Callister 6e. (Fig. 4.12(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].)

37
**AMORPHOUS MATERIALS Crystalline materials...**

• atoms pack in periodic, 3D arrays • typical of: -metals -many ceramics -some polymers crystalline SiO2 Adapted from Fig. 3.18(a), Callister 6e. Noncrystalline materials... • atoms have no periodic packing • occurs for: -complex structures -rapid cooling "Amorphous" = Noncrystalline noncrystalline SiO2 Adapted from Fig. 3.18(b), Callister 6e.

38
**X-RAYS TO CONFIRM CRYSTAL STRUCTURE**

• Incoming X-rays diffract from crystal planes, following Braggs law: nl = 2dsin(q) Adapted from Fig. 3.2W, Callister 6e. • Measurement of: Critical angles, qc, for X-rays provide atomic spacing, d.

39
**SCANNING TUNNELING MICROSCOPY**

• Atoms can be arranged and imaged! Photos produced from the work of C.P. Lutz, Zeppenfeld, and D.M. Eigler. Reprinted with permission from International Business Machines Corporation, copyright 1995. Carbon monoxide molecules arranged on a platinum (111) surface. Iron atoms arranged on a copper (111) surface. These Kanji characters represent the word “atom”.

40
**SUMMARY • Atoms may assemble into crystalline,**

polycrystalline or amorphous structures. • We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). • Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but properties are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains.

41
ANNOUNCEMENTS Reading: Chapter 3

Similar presentations

Presentation is loading. Please wait....

OK

SUMMARY: BONDING Type Bond Energy Comments Ionic Large!

SUMMARY: BONDING Type Bond Energy Comments Ionic Large!

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on event handling in javascript code Ppt on world environment day logo Ppt on international stock exchange Ppt on forward rate agreement notation Ppt on principles of peace building institute of africa Ppt on windows 7 operating system Ppt on hotel industry in india 2013 Ppt on new zealand culture and tradition Ppt on indian travel and tourism Ppt on save environment posters